Metastable Phase Equilibrium in the Aqueous Quaternary System (Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O) at 273.15 K Ying Zeng,*,†,‡ Fujia Cao,† LongGang Li,§ Xudong Yu,† and Xiaofeng Lin|| †
Department of Geochemistry, College of Materials and Chemistry & Chemical Engineering, Chengdu University of Technology, Chengdu 610059, P. R. China ‡ Mineral Resources Chemistry Key Laboratory of Sichuan Higher Education Institutions, Chengdu 610059, P. R. China § The Development and Comprehensive Utilization of Marine Sedimentary Brine, Sichuan Provincial Key Laboratory, Chengdu 610059, P. R. China Panzhihua Steel Corporation, Panzhihua 617067, P. R. China ABSTRACT: The quaternary system (Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O) is one of the most important and basic subsystems of the brines located in the area of the Qinghai-Xizang (Tibet) Plateau. To make certain the solubility of the lithium, sodium, and borate changes with the temperature, the metastable equilibrium of the quaternary system (Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O) was investigated at 273.15 K using an isothermal evaporation method. The solubilities of the equilibrated solution were measured using chemical analytical methods. The crystalloid forms of the solid phase were determined using an X-ray diﬀraction method. This system is of a complex type, with a double salt of sodium and lithium sulfate (3Na2SO4 3 Li2SO4 3 12H2O) formed at 273.15 K. The phase diagram of this system consists of three invariant points, seven univariant curves, and ﬁve crystallization ﬁelds. Comparisons between the phase diagrams of this system at 273.15 K and at 288.15 K show that the crystallization forms and the size of crystallization ﬁeld of salt have changed. The solubility of salt sodium borate changes with temperature more obviously than that of salt lithium borate. Thus, the crystallization area of Na2B4O7 3 10H2O becomes bigger obviously, whereas the crystallization area of salt LiBO2 3 8H2O becomes smaller at 273.15 K. This diﬀerence is beneﬁcial to separate sodium and lithium using an evaporation method, and a rise in temperature is necessary to obtain more lithium borate from the solution.
’ INTRODUCTION A series of salt lakes in the west of China, especially in the area of the Qinghai-Xizang (Tibet) Plateau, are famous for their abundance of lithium and borate resources.1 The main component of these brines can be described as the complex system (Liþ þ Naþ þ Kþ þ Mg2þ þ Cl þ CO32 þ SO42 þ borate anions þ H2O). The evaporation method is often used to exploit the brines and mineral resources. It is well-known that phase equilibria and phase diagrams play an important role in establishing the evaporation process. Earlier researchers found that in the evaporation process of brine the equilibria among the salts are always metastable,2,3 and therefore, more attention has been focused on the investigation of metastable phase equilibrium and metastable phase diagram. So far, a lot of work has been done on metastable phase equilibria aimed at diﬀerent types of brines. The metastable phase equilibria of the seawater system (Naþ þ Kþ þ Mg2þ þ Cl þ SO42 þ H2O) were studied at 288.15 K,4,5 298.15 K,6 and 308.15 K7 using an isothermal evaporating method; the metastable phase equilibria of the sulfate salt lake brines system (Liþ þ Mg2þ þ Cl þ SO42 þ H2O) were studied at 298.15 K;8 and the metastable phase equilibria of the carbonate salt lake brines were studied at 288.15 K and 298.15 K.9,10 These research results, especially the research results of the seawater system (Naþ þ Kþ þ Mg2þ þ Cl þ SO42 þ H2O), have been widely used in the industrial process of salt production, such as extracting schoenite (MgSO4 3 K2SO4 3 6H2O) or potassium r 2011 American Chemical Society
sulfate (K2SO4) from the Chaidamu Saline Lake, China. However, most of the eﬀort has focused on temperatures above 288.15 K, including our earlier work aimed at the Zabuye Salt Lake, located at Qinghai-Xizang (Tibet) Plateau.9,10 The quaternary system (Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O) is one of the most important and basic subsystems of the complex system mentioned above. The metastable phase equilibria of this system have been studied at 288.15 K,11 whereas the metastable phase equilibria of this system at other temperatures are not reported in the literature yet. To make certain the solubility of the lithium, sodium, and borate changes with the temperature, the metastable equilibria of the quaternary system (Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O) at 273.15 K were investigated. The solubilities and densities of the equilibria solution of this system were measured, and the comparisons between the phase diagram at 273.15 K and 288.15 K have also been made.
’ EXPERIMENTAL SECTION Reagents and Apparatus. The chemicals used in this work were of analytical grade purity and from the Peking Xinhua Received: January 25, 2011 Accepted: March 16, 2011 Published: March 29, 2011 2569
dx.doi.org/10.1021/je200091k | J. Chem. Eng. Data 2011, 56, 2569–2573
Journal of Chemical & Engineering Data Chemical Reagent Plant. They were sodium sulfate (Na2SO4, 99.0 % (w/w)), lithium sulfate (Li2SO4, 99.0 % (w/w)), sodium borate (Na2B4O7 3 10H2O, 99.5 % (w/w)), and lithium borate (Li2B4O7, 99.5 % (w/w)). Doubly deionized water was obtained from a Millipore water system with an electrical conductivity less than 1 3 104 S 3 m1 and pH = 6.6. For each experiment, the required amounts of the reagents were dissolved in enough deionized water to produce the experimental solutions. A SHH-250 type thermostatic evaporator made by the Chongqing INBORN Instrument Corporation, China, was used for the metastable phase equilibrium experiments. The equipment has a temperature-controlling apparatus with a blower accessory to control the temperature and the evaporation quantity of the evaporating system. The evaporation rate is (4.0 to 5.5) mm 3 d1, the temperature with an operating range of (258.15 to 373.15) K, and the temperature precision is ( 0.1 K. A DX-2700 X-ray diﬀractometer with Cu KR radiation was used to analyze the crystalloid form of the solid phases. The operating conditions were 40 kV and 30 mA. A standard analytical balance of 110 g capacity and 0.0001 g resolution (AL104, supplied by Mettler Toledo Instruments Co., Ltd.) was employed for the determination of the density of solution. An inductively coupled plasma optical emission spectrometer (ICP-OES, Type Optima5300V) made by P.E. Corporation, U.S.A., was employed for the determination of lithium and sodium ion concentration in solution. Experimental Method. The isothermal evaporation method was employed in this study. The required amounts of reagent, calculated according to the solubility of the salt at 273.15 K and the solubility data of the invariant point of the ternary subsystem, were dissolved into 1000 mL of deionized water to produce the initial evaporating solutions. A series of prepared experimental solutions of the quaternary system were loaded into clean opened polyethylene containers (24 cm long, 14 cm wide, and 7 cm high). The containers were placed in a thermostatic evaporator. The temperature of the solution inside the evaporator was controlled to (273.15 ( 0.1) K and measured by a J thermocouple with an operating range of (258.15 to 373.15) K and a system precision of ( 0.1 K. When enough new solid appeared in the evaporating containers, the liquid and solid phases were separated by filtration. The obtained wet crystals in the solid phase were dried at 273.15 K, pestled into a powder, and then analyzed by X-ray diffraction to determine the crystalloid form of the solid phase. At the same time, a 5.0 mL sample of the clarified solution was taken from the liquid phase and diluted to a 50 mL final volume in a volumetric flask filled with deionized water to analyze the concentration of liquid-phase components. Another 5.0 mL sample of the clarified solution was taken to determine the density. The remainder of the solution was loaded back into the polyethylene containers, placed in the thermostatic evaporator, and continued to be evaporated to reach the next measuring point. This same procedure was repeated until the solution was fully evaporated. The densities of solution were determined in this study and used for the mass fraction calculation of liquid components. The speciﬁc gravity bottle method with correction of air ﬂoating force was used. The precision of the density measure was 0.0001 g 3 cm3. The sample was obtained at 273.15 K and measured at 293.15 K. The excursion caused by the temperature diﬀerence was calibrated by using a multipoint temperature revision method.12
Analytical Methods. The sulfate ion concentration was determined by titration with a standard solution of EDTA in the presence of an excess BaMg mixture solution. First, excess of a BaMg mixture solution (contents 0.01 mol 3 L1 BaCl2 and 0.005 mol 3 L1 MgCl2) was added quantitatively to give a BaSO4 precipitate. The excess BaCl2 solution was then titrated with EDTA standard solution in the presence of mixed KB (Acid chrome blue KNaphthol green B) indicator. The precision of the measurements was better than 0.5 %. The ion concentration measurement was repeated up to three times to estimate the reproducibility. The borate ion concentration was determined by neutralization titration in the presence of propanetriol (precision: ( 0.3 %).13 Boric acid is a weak acid and only partially neutralized by direct titration with a sodium hydroxide standard solution. To improve the measure accuracy, an appropriate amount of polyhydric alcohol like propanetrial is added into the solution before titration to form boron hydroxyl complexes with high dissociation constant. The sodium and lithium ion concentration was determined by inductively coupled plasma optical emission spectrometry, with the precision less than 0.06 %.
’ RESULTS AND DISCUSSION Phase Diagram at 273.15 K. The experimental results of solubilities and densities for the quaternary system Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O at 273.15 K were measured and are tabulated in Table 1. In Table 1, w(B) is the mass fraction of B, and n(B) is the mole number of B, with n(Li22þ) þ n(Na22þ) = n(B4O72) þ n(SO42) = 100 mol. J(B) is the Jan€ecke index values of B, with J(Li22þ) þ J(Na22þ) = J(B4O72) þ J(SO42) = 100. The calculating formula for J(B) is
nðBÞ 100 nðLi2 2þ Þ þ nðNa2 2þ Þ 3
The calculating formula for water concentration is JðH2 OÞ ¼
wðH2 OÞ 100 18 3 ½nðLi2 2þ Þ þ nðNa2 2þ Þ 3
With the data of the Jan€ecke index J(B), the experimental solubility isothermal metastable phase diagram of the system at 273.15 K was constructed, as shown in Figure 1. The metastable equilibrium phase diagram of the system Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O at 273.15 K consists of ﬁve crystallization ﬁelds, seven univariant curves, and three invariant points. The ﬁve crystallization ﬁelds correspond to four single salts, LiBO2 3 8H2O, Na2B4O7 3 10H2O, Na2SO4 3 10H2O, and Li2SO4 3 H2O, and one double salt, 3Na2SO4 3 Li2SO4 3 12H2O. The seven univariant curves, namely, curves AE3, BE3, CE1, DE1, EE2, E1E2, and E2E3, are cosaturated with two salts, respectively. There are four ternary subsystems of the quaternary system Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O that are ternary systems Li2SO4 þ Na2SO4 þ H2O, Li2B4O7 þ Na2B4O7 þ H2O, Li2SO4 þ Li2B4O7 þ H2O, and Na2SO4 þ Na2B4O7 þ H2O. In Figure 1, points A, B, C, D, and E are ﬁve invariant points of the four ternary systems of this quaternary system, cosaturated with two salts, respectively. Among these four ternary systems, system Li2SO4 þ Na2SO4 þ H2O is of a complex type, has two invariant points D and E, with the double salt 3Na2SO4 3 Li2SO4 3 2570
dx.doi.org/10.1021/je200091k |J. Chem. Eng. Data 2011, 56, 2569–2573
Journal of Chemical & Engineering Data
Table 1. Experimental Values of Solubility and Density of the Equilibrium Solution in the Quaternary System Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O at 273.15 Ka composition of solution, w(B) 3 102
Jan€ecke index of dry salt J(Li22þ) þ J(Na22þ) = J(SO42) þ J(B4O72) = 100
w(Naþ) w(B4O72) w(SO42) w(Liþ) w(H2O)
(g 3 cm3)
LiS þ LiB
LiS þ LiB
LiS þ LiB þ NaB LiBþ NaB
NaBþ NaS NaBþ NaS
NaBþ NaSþ NaLiS
NaLiS þ LiS
NaLiS þ LiS þ NaB
Note: NaSNa2SO4 3 10H2O, LiSLi2SO4 3 H2O, NaLiS3Na2SO4 3 Li2SO4 3 12H2O, NaBNa2B4O7 3 10H2O, LiBLiBO2 3 8H2O.
Figure 1. Metastable phase equilibrium diagram of the quaternary system Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O at 273.15 K.
12H2O formed. The double salt 3Na2SO4 3 Li2SO4 3 12H2O is also found in the investigated quaternary system. There are three invariant points in Figure 1, labeled as E1, E2, and E3. The invariant points are cosaturated with three salts, and the equilibrated solid phases of the invariant points were conﬁrmed with X-ray diﬀraction analysis. Figure 2 gives the X-ray diﬀraction pattern of the invariant point E2, which is saturated with salts Li2SO4 3 H2O, Na2B4O7 3 10H2O, and 3Na2SO4 3 Li2SO4 3 12H2O. Figure 3 gives the X-ray diﬀraction pattern of the invariant point E3, which is saturated with salts Li2SO4 3 H2O, Na2B4O7 3 10H2O and LiBO2 3 8H2O. The saturated salts and the mass fraction composition for the three invariant points are listed below.
Figure 2. X-ray diﬀraction pattern of the invariant point E2 (Na2B4O7 3 10H2O þ Li2SO4 3 H2O þ 3Na2SO4 3 Li2SO4 3 12H2O).
Point E1 is saturated with salts Na2SO4 3 10H2O þ 3Na2SO4 3 Li2SO4 3 12H2O þ Na2B4O7 3 10H2O. The mass fraction composition of the corresponding liquid phase is w(Naþ) = 1.49 %, w(Liþ) = 1.06 %, w(B4O72) = 0.89 %, and w(SO42) = 9.91 %. Point E2 is saturated with salts Li2SO4 3 H2O þ 3Na2SO4 3 Li2SO4 3 12H2O þ Na2B4O7 3 10H2O. The mass fraction composition of the corresponding liquid phase is w(Naþ) = 2.43 %, w(Liþ) = 3.28 %, w(B4O72) = 3.12 %, and w(SO42) = 27.64 %. Point E3 is saturated with salts Li2SO4 3 H2O þ Na2B4O7 3 10 H2O þ LiBO2 3 8H2O. The mass fraction composition of the corresponding liquid phase is w(Naþ) = 1.06 %, w(Liþ) = 3.61 %, w(B4O72) = 1.85 %, and w(SO42) = 26.03 %. 2571
dx.doi.org/10.1021/je200091k |J. Chem. Eng. Data 2011, 56, 2569–2573
Journal of Chemical & Engineering Data The crystallization ﬁeld of the salt Na2B4O7 3 10H2O is the largest, which indicates that sodium borate is easier to saturate
Figure 3. X-ray diﬀraction pattern of the invariant point E3 (LiBO2 3 8H2O þ Li2SO4 3 H2O þ Na2B4O7 3 10H2O).
Figure 4. Density vs composition diagram of the quaternary system Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O at 273.15 K.
and crystallize than the other four salts from solution at the investigated temperature. In Figure 4, the ordinate is the density of equilibrated solution, and the abscissa is the mass fraction of lithium. Figure 4 shows that the density changes regularly with the composition of lithium in the solution. In this system, the solubility of lithium sulfate is greater than that of the other salts; therefore, the concentration of lithium sulfate is the main factor aﬀecting the solution density. The density increases with the increase of concentration of lithium and reaches a maximum value at the invariant point E3. At the univariant curves CE1 and BE3 (cosaturated with salt lithium borate and sodium borate and salt sodium sulfate and sodium borate, respectively), because of the rapid condensing of salt Li2SO4, the density of the solution varies with greater range along with the change of lithium composition, while at the other univariant curves, the density of the solution varies with lesser range. The water content diagram of the system is constructed in Figure 5. In Figure 5, the ordinate is the J€anecke index of water (mol H2O/100 mol dry salt), and the abscissa is the mass fraction of lithium. Figure 5 shows that the water content changes regularly with a composition of lithium ion and reaches the smallest value at the invariant point E3. At the univariant curves CE1 and BE3, the solution is dilute and has rapid evaporating rate at the early stage of evaporating. Along with the evaporating process, the evaporating rate is slowed down with an increase of lithium sulfate concentration. Comparison with the Metastable Phase Diagrams at (273.15 and 288.15) K. The matastable phase equilibrium of the quaternary system Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O has been studied at 288.15 K.11 Comparisons between the two phase diagrams at different temperatures shows that the crystallization fields and the crystallization forms have changed. The crystallization form of lithium borate is Li2B4O7 3 3H2O at 288.15 K, whereas that is lithium metaborate (LiBO2 3 8H2O) at 273.15 K, with the crystallization forms Li[B(OH)4] 3 6H2O, as shown in Figure 3. The crystallization form of sodium sulfate has also changed; it is Na2SO4 3 10H2O at 273.15 K, whereas that is Na2SO4 at 288.15 K. Although the double salt of sodium and lithium sulfate is formed in the quaternary system both at 273.15 K and at 288.15 K, the crystallization form of the double salt has changed from Na2SO4 3 Li2SO4 at 288.15 K to 3Na2SO4 3 Li2SO4 3 12H2O at 273.15 K. The metastable phase diagrams of this quaternary system at diﬀerent temperatures all have three invariant points. The mass
Figure 5. Water-content diagram of the quaternary system Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O at 273.15 K. 2572
dx.doi.org/10.1021/je200091k |J. Chem. Eng. Data 2011, 56, 2569–2573
Journal of Chemical & Engineering Data fraction compositions of the solution and the solid phases corresponding with the three invariant points have obviously changed. At 288.15 K, the three invariant points all saturated with salt Li2B4O7 3 3H2O, while at 273.15 K, with the crystallization ﬁeld of salt LiBO2 3 8H2O becoming smaller and that of salt Na2B4O7 3 10H2O becoming larger, there is only one invariant point saturated with salt LiBO2 3 8H2O. The results show that the solubility of salt sodium borate changes with temperature more obviously than that of salt lithium borate. This information can be used to separate sodium borate and lithium borate.
’ CONCLUSION Metastable phase equilibrium in the quaternary system Li2SO4 þ Na2SO4 þ Li2B4O7 þ Na2B4O7 þ H2O was investigated at 273.15 K using an isothermal evaporation method. Solubilities and densities of the solution were determined experimentally. On the basis of the experimental data, the metastable phase diagram, the water content diagram, and the density vs composition diagram were constructed. This system is of a complex type, and the double salt of sodium and lithium borate is formed at the investigated temperature. There are three invariant points, seven univariant curves, and ﬁve crystallization ﬁelds in the metastable phase diagram. The ﬁve crystallization ﬁelds correspond to sodium sulfate decahydrate (Na2SO4 3 10H2O), lithium sulfate monohydrate (Li2SO4 3 H2O), sodium tetraborate decahydrate (borax, Na2B4O7 3 10H2O), lithium metaborate octahydrate (LiBO2 3 8H2O), and a sodium and lithium sulfate double salt (3Na2SO4 3 Li2SO4 3 12H2O), respectively. The salt borax has the largest crystallization ﬁeld and can be easily separated from the solution at 273.15 K. Comparisons between the phase diagram at 273.15 K and the one at 288.15 K show that the crystallization forms and crystallization ﬁelds of the salts in this system change with temperature, and the solubility of salts changes obviously with temperature. This result is beneﬁcial to separate the sodium and lithium borate from the investigated system.
(5) Jin, Z. M.; Zhou, H. N.; Wang, L. S. Studies on the Metastable Phase Equilibrium of Naþ, Kþ, Mg2þ/Cl, SO42--H2O Quinary System at 288 K. Chem. J. Chin. Univ. 2002, 23, 690–694. (6) Jin, Z. M.; Xiao, X. Z.; Liang, S. M. Study of the Metastable Equilibrium for Quinary System of (Naþ, Kþ, Mg2þ), (Cl, SO42-), H2O. Acta Chim. Sin. 1980, 38, 313–321. (7) Jin, Z. M.; Zhou, H. N.; Wang, L. S. Studies on the Metastable Phase Equilibrium of (Naþ, Kþ, Mg2þ), (Cl, SO42-), H2O Quinary System at 308.15 K. Chem. J. Chin. Univ. 2001, 22, 634–638. (8) Guo, Z. Z.; Liu, Z. Q.; Chen, J. Q. Metastable Phase Equilibrium of Liþ, Mg2þ//Cl, SO42—H2O Quaternary System at 298 K. Acta Chim. Sin. 1991, 49, 937–943. (9) Yan, S. Y.; Chen, T.; Liang, Q.; Yin, H. A.; Zeng, Y. Studies on the Reciprocal Quaternary System Liþ, Kþ//CO32-, B4O72- -H2O at 298 K. Chin. J. Inorg. Chem. 2008, 24, 1164–1167. (10) Zeng, Y.; Shao, M. Liquid-solid metastable equilibria in the quinary system Liþ þ Kþ þ Cl þ CO32- þ B4O72- þ H2O at T = 288 K. J. Chem. Eng. Data 2006, 51, 219–222. (11) Sang, S. H.; Yu, H. Y.; Cai, D. Z. Studies on the Reciprocal Quaternary System Liþ, Naþ//SO42-, B4O72-H2O at 288 K. Chin. J. Inorg. Chem. 2005, 21, 1316–1321. (12) Xu, G. L. The Determination and Application of the Temperature Correction Coeﬃcient for the Density of Vinyl Acetate. Fujian Anal. Test. 1999, 3, 1104–1108. (13) Institute of Qinghai Salt-Lake of Chinese Academy of Sciences. Analytical Methods of Brines and Salts, 2nd ed.; Chinese Science Press: Beijing, China, 1984.
’ AUTHOR INFORMATION Corresponding Author
*E-mail: [email protected]
Financial support for this work was provided by the National Nature Science Foundation of China (No. 40673050), the Research Fund for the Doctoral Program of Higher Education from the Ministry of Education of China (Grant 20070616008), the Scholarship Leaders Training Fund from Sichuan Province, and the Project of China Geological Survey (Grant 1212010011809).
’ REFERENCES (1) Zheng, M. P.; Liu, W. G.; Xiang, J. Qinghai-Xizhang Plateau Saline Lakes; Beijing Science and Technology Press: Beijing, China, 1989. (2) Lepeshko, I. N.; Romaschova, N. N. Solubility in system Li2SO4 Na2SO4MgSO4H2O at 298 K. J. Inorg. Chem. 1959, 12, 2812–2815 (in Russian). (3) Gao, S. Y.; Song, P. S.; Xia, S. P.; Zheng, M. P. Chemistry of Salt Lakes New Salt Lake of Boron and Lithium; Beijing Science and Technology Press: Beijing, China, 2007. (4) Shu, Y. G.; Li, J.; Jiang, C. F. Studies on the Metastable Phase Equilibrium of Naþ, Kþ, Mg2þ/Cl, SO42--H2O Quinary System at 288 K. J. Chem. Ind. Eng. Chin. 1992, 43, 549–555. 2573
dx.doi.org/10.1021/je200091k |J. Chem. Eng. Data 2011, 56, 2569–2573